Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

PAPER

Cite this: Nanoscale, 2014, 6, 3259

View Journal | View Issue

Quantum phase transitions and topological proximity eﬀects in graphene nanoribbon heterostructures Gufeng Zhang,abc Xiaoguang Li,*abd Guangfen Wu,ad Jie Wang,a Dimitrie Culcer,ae Efthimios Kaxirasf and Zhenyu Zhang*a Topological insulators are bulk insulators that possess robust chiral conducting states along their interfaces with normal insulators. A tremendous research eﬀort has recently been devoted to topological insulatorbased heterostructures, in which conventional proximity eﬀects give rise to a series of exotic physical phenomena. Here we establish the potential existence of topological proximity eﬀects at the interface between a topological insulator and a normal insulator, using graphene-based heterostructures as prototypical

systems.

Unlike

conventional

proximity

eﬀects

in

topological

insulator

based

heterostructures, which refer to various phase transitions associated with the symmetry breaking of speciﬁc local order parameters, topological proximity eﬀects describe the rich variety of quantum phase transitions associated with the global properties of the system measured by the location of the topological edge states. Speciﬁcally, we show that the location of the topological edge states exhibits a versatile tunability as a function of the interface orientation, the strength of the interface tunnel coupling between a topological graphene nanoribbon and a normal graphene nanoribbon, the spin–orbit coupling strength in the normal graphene nanoribbon, and the width of the system. For zigzag and bearded graphene nanoribbons, the topological edge states can be tuned to be either at the interface or outer edge of the normal ribbon. For armchair graphene nanoribbons, the potential location of the topological edge state can be further shifted to the edge of or within the normal ribbon, to the interface, or diving into the topological graphene nanoribbon. We further show that the topological phase diagram Received 4th October 2013 Accepted 25th December 2013

established for the prototypical graphene heterostructures can also explain the intriguing quantum phase

DOI: 10.1039/c3nr05284b

transition reported recently in other topological-insulator heterostructures. We also discuss potential experimental realizations of the predicted topological proximity eﬀects, which may pave the way for

www.rsc.org/nanoscale

integrating the salient functionality of topological insulators and graphene in future device applications.

1

Introduction

The discovery of topological insulators (TIs) has revolutionized our understanding of insulating behavior.1–11 The appearance of topologically insulating behavior is associated with a topological phase transition.1,3,12,13 For example, when the spin–orbit coupling (SOC) exceeds a critical strength, a band inversion

a

International Center for Quantum Design of Functional Materials(ICQD), Hefei National Laboratory for Physical Sciences at the Microscale, University of Science and Technology of China, Hefei, Anhui, 230026, China. E-mail: [email protected]; [email protected]

b

State Key Laboratory of Surface Physics and Department of Physics, Fudan University, Shanghai, 200433, China

c

Department of Physics, University of California, San Diego, La Jolla, CA 92093, USA

d

Shenzhen Institutes of Advanced Technology, Chinese Academy of Sciences, Shenzhen, 518055, China

e

School of Physics, The University of New South Wales, Sydney 2052, Australia

f

School of Applied Science and Engineering, Harvard University, Cambridge, MA 02138, USA

This journal is © The Royal Society of Chemistry 2014

takes place, rendering the entire system topologically nontrivial. Topological phase transitions do not involve symmetry breaking, but entail instead a change in the Z2 topological invariant, which may be regarded as a quantity counting the number of Dirac cones. No local order parameters can be dened for a topological phase transition: such TI behavior, which is protected against time-reversal invariant perturbations, is a one-particle phenomenon and is the result of SOC. The carriers at the interface between a TI and a normal insulator are massless Dirac fermions with spin-momentum locking. At the same time, the eld of TI also provides a unique platform for studying the interplay between strong SOC and electron– electron interaction eﬀects,14,15 as manifested by the existence of exotic quantum phase transitions.14 The robustness of topologically protected surface states may enable hybrid TI heterostructure systems to provide fundamental device improvements as well as potential applications.16 Recently, by using various TI-based heterostructures, emergent properties of topological surface states

Nanoscale, 2014, 6, 3259–3267 | 3259

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Nanoscale

have been demonstrated.17–22 For instance, TI forms a natural heterostructure with ordinary insulators,17 which can be used to manipulate topological states and the bulk band gap. By putting a ferromagnet on a TI, the inverse spin-galvanic eﬀect18 and giant spin battery eﬀect19 can be realized. Interesting properties are also found in TI heterostructures with magnetic insulators,20 Mott insulators,21 and Bi(111) bilayer.22 In particular, proximity eﬀects in TI heterostructures yield novel phases of matter.23–30 For example, TI/superconductor heterostructures exhibit a superconducting proximity eﬀect oﬀering the possibility of observing Majorana fermions23 and the potential realization of non-Abelian topological quantum computation.31 The quantized electromagnetic response in a TI-ferromagnetic material heterostructure is due to a topological magnetoelectric eﬀect.26,32 Other novel, technologically important properties have also been demonstrated, such as the enhancement of the catalysis process by robust topological surface states in Au-covered TI.25 TI-based heterostructures are thus systems of both fundamental and practical importance.23–28 Harnessing the robust topological surface states entails an accurate understanding and control of their spatial location. Recent rst-principles studies of three-dimensional (3D) TI/ normal insulator heterostructures have demonstrated that the spatial location of the surface states can be shied to the surface of the normal insulator,27,28 and in a certain parameter range can even be shied back into the TI bulk.27 Such studies suggest the possibility of a topological phase transition induced in a normal insulator via topological proximity eﬀects, identied by the topological surface states leaking out into an adjacent material or moving back into the TI. Whereas conventional proximity eﬀects can be described using local order parameters, topological proximity eﬀects involve a topological phase transition for which a local order parameter cannot be dened. In light of this, a practical and highly nontrivial issue to be addressed is the determination of the exact spatial location of the topological surface states in such TI-based heterostructures. In this paper, we choose graphene as a prototype to explore the general features of the topological proximity eﬀects. Graphene is of great interest, since it has a simple honeycomb lattice structure, while possessing numerous intriguing topological phenomena, such as the integer quantum Hall eﬀect,33 anomalous quantum Hall eﬀect,34 and fractional quantum Hall eﬀect.35 In particular, graphene can be turned into a TI once the intrinsic SOC reaches a large enough value.1 Given the ample energy band structure tunability of graphene, it is convenient to use a graphene-based heterostructure as a prototype to systematically investigate the topological proximity eﬀects by considering several crucial parameters of the model system. We expect that the obtained features of topological proximity eﬀects are also suitable for other 2D or 3D TI-based systems, and may be instructive for the design of future TI-based electronic devices. We explore topological proximity eﬀects on topological phase transitions in an important material class of graphene heterostructures36 consisting of a topological graphene nanoribbon (GNR) and a gapped normal GNR. Three diﬀerent

3260 | Nanoscale, 2014, 6, 3259–3267

Paper

Graphene ribbon geometry with zigzag, bearded and armchair edges. The dashed lines along the zigzag, armchair, and bearded edges labeled with N, M, and Q indicate the Nth, Mth and Qth unit cell in y, x and y directions, respectively. The width of a ribbon is measured in multiples of the unit cell. Ribbons with zigzag and bearded edged have inﬁnite length in the x direction, and for armchair edges in the y direction. Fig. 1

interface orientations are investigated: zigzag, bearded, and armchair (Fig. 1). Unlike conventional proximity eﬀects, in which a phase transition is accompanied by symmetry breaking measured by a local order parameter, the topological proximity eﬀects introduced here surrounding topological phase transitions do not involve a symmetry breaking process. Instead of a local order parameter, the measurement of such topological proximity eﬀects is the location of the topological edge states (TESs), which is determined in this study as a function of the interface coupling strength, the SOC strength in the normal GNR, and the orientations of the interface. For three diﬀerent interface orientations: zigzag, bearded, and armchair, we demonstrate versatile tunabilities in the location of the TES. For zigzag and bearded37 GNRs, it can be tuned to be either at the interface or the outer edge of the normal GNR. For armchair GNRs, the potential location of the TES is further enriched to be at the edge of or within the normal GNR, at the interface, or diving into the topological GNR. Moreover, the dependence of the TES behaviors on the interface orientation is attributed to the diﬀerent locations of the Dirac points of the TES in k space for diﬀerent heterostructures. Taken together, our ndings illustrate the conceptual complexity as well as richness of the topological proximity eﬀect at TI-based heterostructures. This paper is organized as follows: in Section 2, we introduce the tight binding Kane–Mele model for GNR heterostructures and outline our methodology. In Section 3, we show the tunability of the spatial location of the TES as some key parameters in zigzag, bearded, and armchair GNR heterostructures. Before concluding in Section 5, we mainly discuss and explain diﬀerent TES behaviors for diﬀerent kinds of interface orientations in Section 4, where potential applications and experimental realizations are also presented.

2 Methodology We start with the Kane–Mele model1,2 for GNRs. In the present work, we generalize the systems of interest to explore the

This journal is © The Royal Society of Chemistry 2014

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Paper

Nanoscale

topological proximity eﬀects in hybrid GNR heterostructures consisting of a normal and a topological GNRs. In these systems, we focus on two central parameters: the tunnel coupling at the interface between the GNRs, and the strength of the SOC in the normal GNR. We investigate the spatial location of the TES at the interface between the two GNRs for three diﬀerent interface orientations: zigzag, bearded, and armchair (Fig. 1). These three orientations give rise to qualitatively diﬀerent graphene band structures, and consequently the proximity eﬀects take qualitatively diﬀerent forms. For both the topological and normal GNRs, we use the same tight-binding Hamiltonian as follows, but with diﬀerent specications on the parameters: X † X † X H¼t ci cj þ Vi c†i ci þ ilSO ci s dkj dik cj ; (1) hiji

i˛a;b

hhijii

C†i (ci)

where is the electron creation (annihilation) operator on site i; t is the nearest-neighbor hopping; Va(b) is the on-site energy for the A(B) sublattice; lSO is the intrinsic SOC connecting next-nearest neighbors; s is the Pauli matrix vector; i and j are two next-nearest neighbor sites, k is their unique common nearest neighbor, and the vector dik points from k to i. The band structure of graphene can be qualitatively changed by tuning the coupling parameters in eqn (1). When Va ¼ Vb ¼ Vg/2 and lSO ¼ 0, we can obtain a trivial insulator with the band gap equals to Vg. On the other hand, in a pristine graphene where we have Vg ¼ 0, a nontrivial insulator can be obtained pﬃﬃﬃ with the band gap of 6 3lSO . Essentially, the competing between Vg and lSO determines the topological phase of the graphene. Although the intrinsic SOC in carbon system is too weak to produce a visible nontrivial band gap (100 mK (ref. 1 and 38–40)), many viable approaches have been proposed to enhance this. For example, the impurity-induced, lattice driven SOC can be of at least the same order of magnitude as the atomic SOC;41 certain heavy non-magnetic adatoms such as indium and thallium can enhance the intrinsic SOC gap up to room temperature;38 random adsorption of adatoms can suppress intervalley scattering, which is detrimental to the topological phase, but does not aﬀect the induced SOC, consequently stabilizing the topological phase in graphene.42 All GNR heterostructures we discuss consist of a normal and a topological GNR with the same interface orientation. The width of the GNRs is measured in multiples of the unit cell illustrated in Fig. 1. In the topological GNR, we set the SOC strength as a constant lSO ¼ 0.03t z 0.08 eV, and the on-site energy Vg ¼ 0. In the normal GNR, we assume a nite Vg to open a trivial band gap, and a relatively small lSO, which is not large enough to induce a topological phase transition as the GNR is isolated. The interface tunnel coupling tc appears as the nearestneighbor hopping energy between the normal and topological GNRs; for zigzag GNR heterostructures, the bonds with tunable coupling tc are illustrated by the red lines in Fig. 2(e–h). The heterostrctures are assumed to be innite in the direction parallel to the interface. We thus solve an eﬀective 1D problem by diagonalizing the Hamiltonian in eqn (1) to obtain band structures and the corresponding edge states.

This journal is © The Royal Society of Chemistry 2014

3 Results In this section, we report the results of band structure and spatial locations edge states in the GNR heterostructures with diﬀerent orientations (zigzag, bearded and armchair). In particular, we investigate the way the TES moves in such systems as a result of the interplay of the interface tunneling, the spin–orbit coupling in the normal GNR and the thickness of the normal GNR. Throughout this study, we consider the thickness of topological GNR to be a large enough constant to avoid direct interaction between the topological edge states on the two sides of the structure. Also, we note that for simplicity, we consider a local interface coupling in this paper. Consideration of a continuously changing interface hopping strength gives qualitatively the same results.

3.1

Zigzag graphene nanoribbon heterostructures

3.1.1 How interface tunneling aﬀects the position of topological edge states. We rst investigate GNR heterostructures with zigzag edges. The heterostructure consists of a normal GNR with width Wn ¼ 3, and a topological GNR with width Wt ¼ 30. Originally, the normal zigzag GNR possesses gapless edge states.43 To distinguish between the topological and trivial edge states, we open a band gap in the normal GNR by adding the diﬀerent on-site energy for the two sublattices. In Fig. 2(a–d), we exhibit a series of band structures of systems with the diﬀerent interface coupling tc, while the xed on-site energy Va ¼ Vb ¼ 0.1t and SOC strength lSO ¼ 0 in the normal GNR. E1 and E2 represent the energy of trivial edge states, which locate separately at the edges of the normal GNR, and the Dirac points (denoted as D1 and D2) describing the band crossing of the TESs to emphasize the linear dispersion around the corresponding k point. We also show spin orientations near the Fermi level in Fig. 2(b–d) with spin up in blue and spin down in red. Based on our denition, the electrons of E2 and D1 are located near the interface between the normal and topological GNRs, and therefore are more sensitive to the tunnel coupling tc. As we gradually increase tc as illustrated in Fig. 2 from le to right, both the energies and spatial locations of these edge states will change accordingly. To see the evolution of the states clearly, we analyze the transition as follows: tc/t ¼ 0 (Fig. 2(a) and (e)). The two GNRs are detached, and the two Dirac points are degenerate. The state D1 is located at the interface of the heterostructure, as shown by the blue area in Fig. 2(e). tc/t ¼ 0.2 (Fig. 2(b) and (f)). As tc increases, the interaction between bands D1 and E2 results in the energy of D1 increasing and that of E2 decreasing. But the spatial location of D1 does not change. tc/t ¼ 0.32 (Fig. 2(c) and (g)). The energy of D1 increases to slightly exceed E1. The spatial location of D1 stays at the interface. tc/t ¼ 0.45 (Fig. 2(d) and (h)). The topological phase transition happens when the bands E1 and D1 detach. Now D1 becomes the at band with energy lower than E1, and its spatial location moves to the outer edge of the normal GNR (Fig. 2(h)).

Nanoscale, 2014, 6, 3259–3267 | 3261

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Nanoscale

Paper

Fig. 2 Band structures of zigzag edge GNR heterostructures (Wn ¼ 3, Wt ¼ 30) for diﬀerent tunnel coupling strengths (a–d), and the corresponding spatial locations of higher energy Dirac points (denoted as D1 in (a–d)) are shown by blue areas in (e–h). Diﬀerent spin orientations are shown as spin up (blue) and spin down (red) near Fermi levels in band structures. The interface tunnel coupling tc ¼ 0 in (a) and (e), tc ¼ 0.2t in (b) and (f), tc ¼ 0.32t in (c) and (g), tc ¼ 0.45t in (d) and (h). For the normal GNR, Vg ¼ 0.1t and lSO ¼ 0; for the topological GNR, Vg ¼ 0 and lSO ¼ 0.03t. E1 and E2: the bands of the trivial edge states originated from the normal GNR. D2: the other Dirac point whose spatial location is far away from the interface. Dashed lines in (e–h) indicate the interface of the heterostructures, and the red bonds show the interface tunnel coupling (tc).

Aer the phase transition, further increasing tc will not change the energy and spatial location of D1, but will keep enlarging the energy of E1 and reducing the energy of E2 toward bulk states, implying that these two states are spatially more close now. In the whole process, the energy of D2 does not change, because its spatial location is far away from the interface. For very large tc, E1 and E2 are mixed with bulk states, and we can see only two TESs located separately at two edges of the whole heterostructures. The shi of TESs from the interface to the outer edge of the normal GNR indicates that the

Fig. 3 Phase diagram for zigzag GNR heterostructures, spanned by the tunnel coupling (tc) and SOC in the normal GNR. The black solid line indicates the boundary of P1 and P2 phases with Wn ¼ 3, Wt ¼ 30. Insets are the illustrations of the spatial locations of the TESs. P1 phase: the TES is located at the interface. P2 phase: the TES is located at the outer edge of the normal GNR.

3262 | Nanoscale, 2014, 6, 3259–3267

heterostructure in its entirety becomes an expanded 2D TI via the topological proximity eﬀect. 3.1.2 How spin–orbit coupling aﬀects the position of topological edges states. Qualitatively similar pictures are observed when we include a nite SOC in the normal GNR. Under the inuence of both the tunnel coupling and SOC, the system still has two phases. As shown in the phase diagram Fig. 3, the phase transition occurs at the boundary of the P1 and P2 areas. Specically, for given values of t and lSO, tc separating the two phases decreases monotonically as the SOC in the normal GNR increases. In other words, the SOC in the normal GNR helps the transition happen. We can understand this physical picture by considering the limiting case when we apply a large enough SOC in the normal GNR to induce the topological phase transition without the presence of other topological proximities. In this case, the TES will not appear at the interface (P1 phase) for any nite tc, but at the edges of the whole heterostructure (P2 phase), because both GNRs are topologically nontrivial. 3.1.3 Whole phase diagram of the position of topological edge states. Furthermore, we discuss the way the width of the normal GNR aﬀects the phase transition. Fig. 4 shows the phase diagram for normal GNR with diﬀerent widths Wn ¼ 3, 10, 15, 20, 25. We see that for the same SOC in the normal GNR, the wider one requires a larger tunnel coupling tc to induce the transition from P1 to P2. This is because the phase transition essentially needs the coupling between the states at the interface and outer edge of the normal GNR, and this coupling becomes weaker as the width increases. So a larger tunnel coupling tc is required to propagate the TESs to further position. In an limiting case where the normal ribbon has innite width, topological proximity eﬀect will not occur for any nite tunnel coupling tc.

This journal is © The Royal Society of Chemistry 2014

View Article Online

Paper

Nanoscale

moves from the interface (P1 phase) to the outer edge of the normal ribbon (P2 phase) [Fig. 5]. Furthermore, switching on the SOC in the normal GNR still preserves the two phases for the TES. The inuence of SOC in normal GNR on the topological proximity eﬀect is the same as in the zigzag case.

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

3.3

Phase diagram for zigzag GNR heterostructures with diﬀerent normal GNR widths, spanned by the tunnel coupling (tc) and SOC in the normal GNR. The lines indicate the boundary of the P1 and P2 phases, which are deﬁned the same as in Fig. 3. We use diﬀerent colors for various widths, as shown in the inset. Fig. 4

In summary for the zigzag GNR heterostructures, two phases exist with diﬀerent tunnel coupling and SOC in the normal GNR: the TES may be located at the interface or at the outer edge of the normal GNR. 3.2

Bearded graphene nanoribbon heterostructures

We now consider bearded edge graphene nanoribbon37 heterostructures. Similar to zigzag GNR, a bearded GNR has gapless trivial edge states. Aer turning on the SOC, a Dirac point emerges at G point (k ¼ 0) [Fig. 8(b)]. We show the topological phase diagram of the bearded edge GNR heterostructure in Fig. 5. The system consists of a normal GNR with width Wn ¼ 3 and topological GNR Wt ¼ 30. As one increases the interface tunnel strength (tc) between the heterostructures, the TES

Armchair graphene nanoribbon heterostructures

Armchair edge GNR heterostructures diﬀer a lot from both zigzag and bearded edge systems in that a pristine (i.e. without SOC) armchair GNR does not have trivial edge states.43 We rst investigate the spatial location of the TES as the tunnel coupling tc increases for the xed SOC in the normal GNR. Fig. 6 displays our calculation results for three SOC values in the normal GNR: (a) no SOC; (b) moderate SOC (lSO/t ¼ 0.02) and (c) strong SOC (lSO/t ¼ 0.06), which is large enough to induce topological phase transition in the normal GNR at tc ¼ 0. In contrast with the zigzag and bearded cases, the armchair GNR heterostructure shows two additional phases in the strong tunnel coupling regime, P3, where the density of the TES peaks in the normal GNR, and P4, where the TES is re-located one unit cell back inside the topological GNR. With no SOC in the normal GNR (a), the location of the TES shis from P1 through P3 to P4 as the coupling increases, while for a moderate SOC (b), the TES can move to the outer edge of the normal GNR through P2 instead of P3 during the evolution. In the limiting case of the strong SOC, the original normal GNR becomes topologically nontrivial. Thus the whole system becomes a 2D TI. With any nite tc, the TES will only exist at the boundary of the whole system as shown in Fig. 6. We note that neither the P3 nor the P4 phase exists for the zigzag or bearded GNR, and the appearance of the P4 phase is consistent with ab initio work reported recently.27 Next, we investigate a series of phase diagram by considering the widths of the normal GNR. Fig. 7 displays the phase diagrams as a function of the tunnel coupling and SOC in the normal GNR for the heterostructures with various normal GNR width Wn and xed topological GNR width Wt ¼ 60. Generally speaking, as tc increases, we see three possible evolution routines for a xed SOC in the normal GNR: P1 / P2 / P4, P1 / P3 / P4, and P2, which correspond to the three subgures in Fig. 6. From Fig. 7, we see clearly that the phase space of P2 extends as the width increases. For a wider normal GNR and large enough SOC, the TESs will not move one unit cell into the topological GNR (P4 phase), but continue to reside at the outer edge of the normal GNR (P2 phase). In such a case, the whole heterostructure acts as a topological insulator which has the TESs on both sides.

4 Discussion Fig. 5 Phase diagram of the TES location without SOC in the normal GNR. The heterostuctures consist of a normal GNR with width Wn ¼ 3 and a topological GNR with width Wt ¼ 30. The dashed line indicates the interface of the heterostructures. P1 phase: the TES is located at the interface. P2 phase: the TES is located at the outer edge of the normal GNR.

This journal is © The Royal Society of Chemistry 2014

The movement of the TES to diﬀerent locations is a manifestation of the complexity of the topological proximity eﬀect. As the interface tunnel coupling becomes stronger, it gets easier for the SOC on the topological side of the junction to leak into the part without SOC, which gives rise to an eﬀective SOC in the normal GNR. However, the phase diagram of the TES locations is diﬀerent for of the GNR heterostructures with diﬀerent

Nanoscale, 2014, 6, 3259–3267 | 3263

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Nanoscale

Paper

Fig. 6 Phase diagram of the TES location for armchair GNR heterostructures with a normal GNR width Wn ¼ 30 on the left and a topological GNR width Wt ¼ 60 on the right. The SOC strength lSO ¼ 0.03t in the topological GNR and is 0 (a), 0.02t (b) and 0.06t (c) in the normal GNR. The onsite energy in the normal GNR is Vg ¼ 0.03t. The dashed lines indicate the interface location. Four phases appear for the TES as the tunnel coupling (tc) increases: P1 phase: the TES is located at the interface; P2 phase: the TES at the outer edge of the normal GNR; P3 phase: the TES in the bulk of the normal GNR; P4 phase: the TES is located one unit cell into the topological GNR.

Fig. 7 Phase diagram for the armchair GNR heterostructures with a topological GNR width Wt ¼ 60 and a normal GNR width Wn ¼ 5 (a), Wn ¼ 10 (b), Wn ¼ 20 (c), Wn ¼ 30 (d), Wn ¼ 40 (e), Wn ¼ 50 (f). All diagrams are spanned by the tunnel coupling (tc/t) and SOC in the normal GNR. The four phases are deﬁned same as in Fig. 6.

orientations. The existence of the trivial edge states in zigzag and bearded heterostructures plays an important role in causing this qualitative diﬀerence. Fig. 8 displays the band structures of the isolated topological GNRs with diﬀerent edge orientations. We note that the Dirac points for the armchair, bearded and zigzag edge GNRs appear at diﬀerent k points. For the zigzag (bearded) edge GNR, the Dirac point at M(G) point is energetically far away from the bulk states. Consequently, the TES at the M(G) points prefers to mix with the edge states in

3264 | Nanoscale, 2014, 6, 3259–3267

normal GNR, which is energetically close to the TES, therefore this rules out the existence of the P3 and P4 phases. However, for the armchair edge GNR, the energy of the Dirac point is close to the bulk bands and the trivial edge state does not exist. As a consequence, it is possible for the TES to interact with the bulk states and move into the bulk, providing the tow more phases P3 and P4 related to the bulk states. In reality, most known TIs have similar band structures to armchair GNRs, namely, the Dirac points of the TES are located

This journal is © The Royal Society of Chemistry 2014

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Paper

Nanoscale

Fig. 8 Band structures of an armchair (a), bearded (b), and zigzag (c) topological GNRs with the widths Wt ¼ 30.

at the same k point as the bulk band gap (Fig. 8(a)). We thus expect that the phase diagram of the armchair GNR heterostructure is also applicable to the similar TI-based heterostructures. In a recent ab initio study, Wu et al.27 have observed in 3D TI/normal insulator heterostructures that the spatial location of the topological surface states can be located at the interface, shied to the surface of the normal insulator, or back into the TI bulk, which corresponds to P1, P2, and P4 in our phase diagram, respectively. On the other hand, the new discovered P3 phase in this study can be expected in the TI/ normal insulator heterostructures with a relatively thick normal insulator layer. For the zigzag GNR heterostructures, we also expect an analogy between the prototypical graphene system and other 3D TI/normal insulator heterostructures with the similar band structures. At this point, it is worthwhile to emphasize that conventional proximity eﬀects involve the order parameter of a brokensymmetry phase of a host material leaking into an adjacent material, which is driven into a broken symmetry state of the host material as well. In the topological proximity eﬀects demonstrated here, modulations of the SOC and interface tunnel coupling shi the boundary between a normal insulator and a TI, accompanied by topological phase transitions. A fascinating feature of the topological proximity eﬀects is the dual-proximity nature: the location of the TES can be switched back and forth between the two materials, including placing the topological phase boundary inside an otherwise structurally homogenous material such as the normal insulator or the TI. One can regard a conventional proximity eﬀect as a spatial extension of a broken symmetry state. In contrast, the topological proximity eﬀect refers to inducing chiral surface states in an adjacent material as well as controlling their location, again, without symmetry breaking. Aside from the conceptual advances, the present study may also oﬀer new opportunities in developing spintronic devices and quantum computing. For example, the systems proposed in this work can be used to induce chiral spin-polarized states in a 2D graphene slab at will, which constitutes an ON/OFF switch based on the TES, and can be regarded as a qubit. Such a switch can be controlled by the SOC or the tunnel coupling. As another example, we can further regard the TES as a current loop, and join a square slab of a topological GNR with a square slab of a

This journal is © The Royal Society of Chemistry 2014

normal GNR. Whereas the topological side is always in the ON state, the state of the normal insulator side can be modulated. A spin polarization may then be induced in this qubit by coupling it to a ferromagnet, which would enable control of the quantum anomalous Hall eﬀect, and would also serve as a spin injector into the normal GNR. Although the predicted topological proximity eﬀects are not limited for the graphene systems, as a very promising material for future electronic devices, we would like to briey discuss the potential experimental realization of the topological proximity eﬀects predicted in graphene. Firstly, as we mentioned before, even though the intrinsic SOC in pristine graphene is commonly known to be quite weak, many approaches have been proposed to enhance it.38,41,42 Recent experiment progresses45 reported colossal enhancement of SOC to 2.5 meV in weakly hydrogenated graphene. Secondly, the coupling between a normal and a topological GNR can be eﬀectively tuned by substrate steps, as demonstrated recently in ref. 44, where the resistance from the steps on the SiC substrate was found to rise due to the abrupt variation in potential and doping as the graphene extends over a step. Lastly, the recently predicted 2D organic topological insulators46,47 with a hexagonal lattice and much larger SOC would oﬀer another platform to implement the topological proximity eﬀect predicted here. These and other alternative candidate structural systems may therefore provide test grounds for physical realization of topological phase transitions.

5 Conclusions We have demonstrated the existence of topological proximity eﬀects in GNR heterostructures consisting of a normal and a topological GNR under a variety of experimentally relevant circumstances. For diﬀerent types of edges – zigzag, bearded, and armchair – the location of the TES is a function of the interface tunnel coupling, the SOC strength in the normal GNR and also the width of the normal GNR, demonstrating a rich quantum phase diagram. These ndings pave the way for designing next-generation quantum devices that integrate the functionality of graphene and TI. We also stress that the novel topological proximity eﬀects demonstrated here using the prototypical systems of GNR heterostructures are conceptually

Nanoscale, 2014, 6, 3259–3267 | 3265

View Article Online

Nanoscale

also applicable to heterostructures consisting of a normal insulator and a 3D TI.17,27,28

Acknowledgements

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

This work was supported by NSF of China (Grant nos 91021019 and 11034006), National Basic Research Program of China (Grant no. 2011CB921801), USDOE (Grant no. DE-FG0302ER45958), and USNSF (Grant no. 0906025).

References 1 C. L. Kane and E. J. Mele, Quantum Spin Hall Eﬀect in Graphene, Phys. Rev. Lett., 2005, 95, 226801. 2 C. L. Kane and E. J. Mele, Z2 Topological Order and the Quantum Spin Hall Eﬀect, Phys. Rev. Lett., 2005, 95, 146802. 3 B. A. Bernevig, T. L. Hughes and S. C. Zhang, Quantum Spin Hall Eﬀect and Topological Phase Transition in HgTe Quantum Wells, Science, 2006, 314, 1757. 4 M. K¨ onig, S. Wiedmann, C. Br¨ une, A. Roth, H. Buhmann, L. W. Molenkamp, X. L. Qi and S. C. Zhang, Quantum Spin Hall Insulator State in HgTe Quantum Wells, Science, 2007, 318, 766. 5 L. Fu, C. L. Kane and E. J. Mele, Topological Insulators in Three Dimensions, Phys. Rev. Lett., 2007, 98, 106803. 6 J. E. Moore and L. Balents, Topological invariants of timereversal-invariant band structures, Phys. Rev. B: Condens. Matter Mater. Phys., 2007, 75, 121306. 7 D. Hsieh, D. Qian, L. Wray, Y. Xia, Y. S. Hor, R. J. Cava and M. Z. Hasan, A topological Dirac insulator in a quantum spin Hall phase, Nature, 2008, 452, 970. 8 Y. Xia, D. Qian, D. Hsieh, L. Wray, A. Pal, H. Lin, A. Bansil, D. Grauer, Y. S. Hor, R. J. Cava and M. Z. Hasan, Observation of a large-gap topological-insulator class with a single Dirac cone on the surface, Nat. Phys., 2009, 5, 398. 9 M. Z. Hasan and C. L. Kane, Colloquium: Topological insulators, Rev. Mod. Phys., 2010, 82, 3045. 10 X. L. Qi and S. C. Zhang, Topological insulators and superconductors, Rev. Mod. Phys., 2011, 83, 1057. 11 H. J. Zhang, C. X. Liu, X. L. Qi, X. Dai, Z. Fang and S. C. Zhang, Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface, Nat. Phys., 2009, 5, 438. 12 M. Kim, C. H. Kim, H. Kim and J. lhm, Topological quantum phase transitions driven by external electric elds in Sb2Te3 thin lms, Proc. Natl. Acad. Sci. U. S. A., 2011, 109, 671. 13 Su.-Y. Xu, Y. Xia, L. A. Wray, S. Jia, F. Meier, J. H. Dil, J. Osterwalder, B. Slomski, A. Bansil, H. Lin, R. J. Cava and M. Z. Hasan, Topological Phase Transition and Texture Inversion in a Tunable Topological Insulator, Science, 2011, 332, 560. 14 D. Pesin and L. Balents, Mott physics and band topology in materials with strong spin–orbit interaction, Nature Phys., 2010, 6, 376. 15 D. Culcer, Linear response theory of interacting topological insulators, Phys. Rev. B: Condens. Matter Mater. Phys., 2011, 84, 235411.

3266 | Nanoscale, 2014, 6, 3259–3267

Paper

16 D. Kong and Y. Cui, Opportunities in chemistry and materials science for topological insulators and their nanostructures, Nat. Chem., 2011, 3, 845. 17 J. A. Hutasoit and T. D. Stanescu, Induced spin texture in semiconductor/topological insulator heterostructures, Phys. Rev. B: Condens. Matter Mater. Phys., 2011, 84, 085103; K. Nakayama, K. Eto, Y. Tanaka, T. Sato, S. Souma, T. Takahashi, K. Segawa and Y. Ando, Manipulation of Topological States and the Bulk Band Gap Using Natural Heterostructures of a Topological Insulator, Phys. Rev. Lett., (2012), 109, 236804; J. Kim, J. Kim, K. Kim, and S. Jhi, Topological phase transition in Dirac fermionic heterostructures, arXiv:1206.2953. 18 I. Garate and M. Franz, Inverse Spin-Galvanic Eﬀect in the Interface between a Topological Insulator and a Ferromagnet, Phys. Rev. Lett., 2010, 104, 146802. 19 F. Mahfouzi, B. K. Nikoli, S.-H. Chen and C.-R. Chang, Microwave-driven ferromagnet–topological-insulator heterostructures: The prospect for giant spin battery eﬀect and quantized charge pump devices, Phys. Rev. B: Condens. Matter Mater. Phys., 2010, 82, 195440. 20 W. D. Luo and X.-L. Qi, Massive Dirac surface states in topological insulator/magnetic insulator heterostructures, Phys. Rev. B: Condens. Matter Mater. Phys., 2013, 87, 085431; S. V. Eremeev, V. N. Men'shov, V. V. Tugushev, P. M. Echenique, and E. V. Chulkov, Magnetic proximity eﬀect at the 3D topological insulator/magnetic insulator interface, arXiv:1304.1275v1. 21 S. Ueda, N. Kawakami, and M. Sigrist, Proximity eﬀects in a topological-insulator/Mott-insulator heterostructure, arXiv:1303.2781. 22 T. Hirahara, G. Bihlmayer, Y. Sakamoto, M. Yamada, H. Miyazaki, S. Kimura, S. Blu€ gel and S. Hasegawa, Interfacing 2D and 3D Topological Insulators: Bi(111) Bilayer on Bi2Te3, Phys. Rev. Lett., 2011, 107, 166801; Z. F. Wang, M.-Y. Yao, W. M. Ming, L. Miao, F. F. Zhu, C. H. Liu, C. L. Gao, D. Qian, J.-F. Jia and F. Liu, Creation of helical Dirac fermions by interfacing two gapped systems of ordinary fermions, Nat. Commun., (2013), 4, 1384. 23 L. Fu and C. L. Kane, Superconducting Proximity Eﬀect and Majorana Fermions at the Surface of a Topological Insulator, Phys. Rev. Lett., 2008, 100, 096407. 24 T. D. Stanescu, J. D. Sau, R. M. Lutchyn and S. Das Sarma, Proximity eﬀect at the superconductor–topological insulator interface, Phys. Rev. B: Condens. Matter Mater. Phys., 2010, 81, 241310(R). 25 H. Chen, W. G. Zhu, D. Xiao and Z. Y. Zhang, CO Oxidation Facilitated by Robust Surface States on Au-Covered Topological Insulators, Phys. Rev. Lett., 2011, 107, 056804. 26 X.-L. Qi, R. D. Li, J. D. Zang and S. C. Zhang, Inducing a Magnetic Monopole with Topological Surface States, Science, 2009, 323, 1184. 27 G. F. Wu, H. Chen, Y. Sun, X. G. Li, P. Cui, C. Franchini, J. L. Wang, X. Q. Chen and Z. Y. Zhang, Tuning the vertical location of helical surface states in topological insulator heterostructures via dual-proximity eﬀects, Sci. Rep., 2013, 3, 1233.

This journal is © The Royal Society of Chemistry 2014

View Article Online

Published on 03 January 2014. Downloaded by Northeastern University on 29/09/2014 06:59:00.

Paper

28 Q. F. Zhang, Z. Y. Zhang, Z. Y. Zhu, U. Schwingenschl¨ ogl and Y. Cui, Exotic Topological Insulator States and Topological Phase Transitions in Sb2Se3-Bi2Se3 Heterostructures, ACS Nano, 2012, 6(3), 2345. 29 D. Culcer, Transport in three-dimensional topological insulators: Theory and experiment, Physica E, 2012, 44, 860. 30 Z. Fang, N. Nagaosa, K. S. Takahashi, A. Asamitsu, R. Mathieu, T. Ogasawara, H. Yamada, M. Kawasaki, Y. Tokura and K. Terakura, The Anomalous Hall Eﬀect and Magnetic Monopoles in Momentum Space, Science, 2003, 302, 92. 31 C. Nayak, S. H. Simon, A. Stern, M. Freedman and S. Das Sarma, Non-Abelian anyons and topological quantum computation, Rev. Mod. Phys., 2008, 80, 1083. 32 X.-L. Qi, T. L. Hughes and S. C. Zhang, Topological eld theory of time-reversal invariant insulators, Phys. Rev. B: Condens. Matter Mater. Phys., 2008, 78, 195424. 33 Y. Zhang, Y.-W. Tan, H. L. Stormer and P. Kim, Experimental observation of the quantum Hall eﬀect and Berry's phase in graphene, Nature, 2005, 438, 201; K. S. Novoselov, Z. Jiang, Y. Zhang, S. V. Morozov, H. L. Stormer, U. Zeitler, J. C. Maan, G. S. Boebinger, P. Kim and A. K. Geim, RoomTemperature Quantum Hall Eﬀect in Graphene, Science, 2007, 315, 1379. 34 Z. H. Qiao, S. A. Yang, W. X. Feng, W.-K. Tse, J. Ding, Y. G. Yao, J. Wang and Q. Niu, Quantum anomalous Hall eﬀect in graphene from Rashba and exchange eﬀects, Phys. Rev. B: Condens. Matter Mater. Phys., 2010, 82, 161414. 35 K. I. Bolotin, F. Ghahari, M. D. Shulman, H. L. Stormer and P. Kim, Observation of the fractional quantum Hall eﬀect in graphene, Nature, 2009, 462, 196. 36 O. Shevtsov, P. Carmier, C. Petitjean, C. Groth, D. Carpentier and X. Waintal, Graphene-Based Heterojunction between Two Topological Insulators, Phys. Rev. X, 2012, 2, 031004.

This journal is © The Royal Society of Chemistry 2014

Nanoscale

37 M. Fujita, K. Wakabayashi, K. Nakada and K. Kusakabe, Peculiar Localized State at Zigzag Graphite Edge, J. Phys. Soc. Jpn., 1996, 65, 1920. 38 C. Weeks, J. Hu, J. Alicea, M. Franz and R. Q. Wu, Engineering a Robust Quantum Spin Hall State in Graphene via Adatom Deposition, Phys. Rev. X, 2011, 1, 021001. 39 H. Min, J. E. Hill, N. A. Sinitsyn, B. R. Sahu, L. Kleinman and A. H. MacDonald, Intrinsic and Rashba spin-orbit interactions in graphene sheets, Phys. Rev. B: Condens. Matter Mater. Phys., 2006, 74, 165310. 40 Y. G. Yao, F. Ye, X.-L. Qi, S.-C. Zhang and Z. Fang, Spin-orbit gap of graphene: First-principles calculations, Phys. Rev. B: Condens. Matter Mater. Phys., 2007, 75, 041401(R). 41 A. H. Castro Neto and F. Guinea, Impurity-Induced SpinOrbit Coupling in Graphene, Phys. Rev. Lett., 2009, 103, 026804. 42 H. Jiang, Z. H. Qiao, H. W. Liu, J. R. Shi and Q. Niu, Stabilizing Topological Phases in Graphene via Random Adsorption, Phys. Rev. Lett., 2012, 109, 116803. 43 K. Wakabayashi, M. Fujita, H. Ajiki and M. Sigrist, Electronic and magnetic properties of nanographite ribbons, Phys. Rev. B: Condens. Matter Mater. Phys., 1999, 59, 8271. 44 T. Low, V. Perebeinos, J. Tersoﬀ and Ph. Avouris, Deformation and Scattering in Graphene over Substrate Steps, Phys. Rev. Lett., 2012, 108, 096601. 45 J. Balakrishnan, G. Kok Wai Koon, M. Jaiswal, A. H. Castro ¨ Neto and B. Ozyilmaz, Colossal enhancement of spin–orbit coupling in weakly hydrogenated graphene, Nat. Phys., 2013, 9, 284. 46 Z. F. Wang, Z. Liu and F. Liu, Organic topological insulators in organometallic lattices, Nat. Commun., 2013, 4, 1471. 47 Z. Liu, Z.-F. Wang, J.-W. Mei, Y.-S. Wu and F. Liu, Flat Chern Band in a Two-Dimensional Organometallic Framework, Phys. Rev. Lett., 2013, 110, 106804.

Nanoscale, 2014, 6, 3259–3267 | 3267